Journal of Nanomaterials

Volume 2014 (2014), Article ID 973156, 7 pages

http://dx.doi.org/10.1155/2014/973156

Research Article

CuO-In ₂O ₃ Core-Shell Nanowire Based Chemical Gas Sensors

Xiaoxin Li,¹ Xiaogan Li,¹ Ning Chen,¹ Xinye Li,² Jianwei Zhang,¹ Jun Yu,¹ Jing Wang,¹ and Zhenan Tang¹

¹School of Electronic Science and Technology, Institute for Sensing Technologies, Key Laboratory of Liaoning for Integrated Circuits Technology, Dalian University of Technology, Dalian 116024, China

²School of Materials Science and Engineering, Dalian University of Technology, Dalian 116024, China

Received 31 October 2013; Revised 22 December 2013; Accepted 23 December 2013; Published 9 February 2014

Academic Editor: Jianping Xie

Copyright © 2014 Xiaoxin Li et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

The CuO-In₂O₃ core-shell nanowire was fabricated by a two-step method. The CuO nanowire core (NWs) was firstly grown by the conventional thermal oxidation of Cu meshes at 500°C for 5 hours. Then, the CuO nanowires were immersed into the suspension of amorphous indium hydroxide deposited from the In(AC)₃ solution by ammonia. The CuO nanowires coated with In(OH)₃ were subsequently heated at 600°C to form the crystalline CuO-In₂O₃ core-shell structure, with In₂O₃ nanocrystals uniformly anchored on the CuO nanowires. The gas sensing properties of the formed CuO-In₂O₃ core-shell nanowires were investigated by various reducing gases such as hydrogen, carbon monoxide, and propane at elevated temperature. The sensors using the CuO-In₂O₃ nanowires show improved sensing performance to hydrogen and propane but a suppressed response to carbon monoxide, which could be attributed to the enhanced catalytic properties of CuO with the coated porous In₂O₃ shell and the p-n junction formed at the core-shell interface.

1. Introduction

There is an increasing demand for highly sensitive gas detecting devices in abundant applications ranging from daily life devices to industrial process control. Metal oxide based gas sensors, which rely on change of electrical conductance due to the interaction with the surrounding gas, have been extensively investigated in the past decades [1, 2]. An efficient strategy to improve sensor performance is to adopt the nanostructured sensing materials that have a high surface area to volume ratio and thus a strong interaction happens between the surrounding gas and the material [3–6]. Semiconductor gas sensors show a resistance change upon exposure to toxic and dangerous gases [7, 8]. Among various types of the nanostructured sensing materials, one-dimensional (1D) nanowires (NWs) with high surface area/volume ratio and less agglomerated configuration are advantageous to accomplish high gas sensitivity and rapid response speed [9–11].

Cupric oxide (CuO), with a bandgap of 1.0–1.9 eV, is intrinsically a p-type semiconductor mainly due to the Cu vacancies [12]. Copper oxide nanowires have been extensively studied for gas sensing in recent years. CuO nanowires exhibited good response to reducing gases, making it promising to be developed for an efficient gas sensor [13]. CuO nanowires had been synthesized by various methods such as wet chemical methods [14, 15], templating methods [16, 17], electrospinning [18], or thermal oxidation of copper [19–22]. Chen et al. demonstrated a H₂S sensor using the vertically aligned CuO nanowire. The sensor showed a good selectivity to H₂S compared with the responses to H₂, CO, and NH₃ [23]. Li et al. also reported that CuO NWs based sensor showed high sensitivities to H₂S and the nanowires were synthesized by a template-assisted electrodeposition method [24]. Wang et al. prepared high quality single-crystal CuO nanowire arrays by the thermal oxidation of copper slices. Then the surfaces of CuO nanowires were modified by magnetron-sputtered ZnO nanoparticles. This composite structure effectively enhanced the selectivity of CuO nanowire gas sensor for detection of CO [25].

In this work, we report the sensing properties of the In₂O₃ nanoisland decorated CuO NWs to different reducing gases. The In₂O₃ nanoisland decorated CuO NWs were prepared by a two-step method: thermal-oxidation followed with dip-coating and calcination. The gas sensing properties of CuO-In₂O₃ composite nanowire based sensor have not yet been studied to our best knowledge. An enhancement in the gas sensing properties was observed in accordance with the p-n juction created between these two nanomaterials.

2. Experimental

2.1. Preparation of CuO-In₂O₃ Core-Shell Nanowire

Firstly, the pure CuO nanowires were prepared by the conventional thermal oxidation of copper following the procedures described in literature [19]. The pure copper meshes (thickness: 0.5 mm, diameter: 3 mm and pore diameter: 100 μm, and purity of 99.998%) were polished with sandpaper to remove the oxide layer of the surface and then the copper was washed in ethanol for 5 min by ultrasonic treatment to remove the possible contaminated grease. Finally, they were rinsed using deionized water and dried naturally in oven at room temperature.

The cleaned copper meshes were placed in a quartz boat and heated in a tube furnace in air. The heating-up step was ramped at a speed of 4°C/min until the temperature reached 500°C and then the temperature was constant at 500°C for 5 hours that was found to be optimum for achieving the high quality nanowires. Then the temperature was cooled down also at a ramping speed of 4°C/min.

The CuO-In₂O₃ composite nanowire sensor was prepared by dip-coating method followed by a thermal decomposition as described in Figure 1. 1 mol/L indium acetate aqueous solution and 3 mol/L of ammonia solution were mixed together according to a ratio of 1 : 1 by volume to obtain the milky indium hydroxide suspension. One drop (about 0.5 mL) of as-prepared indium hydroxide milky suspension was then injected by syringe onto the surface of the CuO nanowire fabricated earlier. Then, these coated CuO nanowires were placed in oven to make them fully dry and subsequently were heated at 600°C for 5 hours to obtain the CuO-In₂O₃ core-shell nanowires.

Figure 1: The procedures for making the CuO-In₂O₃ core shell nanowires.

The surface morphology of the two samples was analyzed using scanning electron microscope equipped with an energy dispersed X-ray spectroscopy (SEM-EDX, FEI, USA). EDX spectrum was used to examine the elemental composition of the core-shell nanowires.

2.2. Sensor Fabrication and Measurements

The whole mesh with the obtained CuO-In₂O₃ core-shell nanostructure on top surface was placed onto a commercial interdigitated gold electrode with the alumina as the substrate. Then a clean alumina brick was put on the top of the mesh to ensure a good contact between the nanowires and the gold electrodes as shown in Figure 2.

Figure 2: Schematic view of the sensor using the CuO-based nanowires. The alumina tile was used to make a good contact between the nanowire arrays with the gold electrodes.

The sensing measurements were conducted in a conventional gas flow apparatus. The electrical resistance of the sensors was measured by a computer controlled Agilent multimeter (100 M, Agilent 34405A). During the electrical measurement, commercially supplied certified gases containing 1500 ppm of CO, C₃H₈ and 4 vol% H₂ in nitrogen, and pure oxygen were diluted by nitrogen, respectively, to obtain different concentrations of the test gases in various oxygen backgrounds. The total gas flow rate was maintained at 250 sccm/min and the flow rate of different gases was controlled independently using computer controlled, precalibrated, electronic mass flow controllers (D07-19B, Beijing Senvenstar Electronics, China). The sensitivity () of a gas sensor is calculated as follows:

where and are resistance of a sensor in air and in detected gas, respectively.

3. Results and Discussion

3.1. Nanowires Synthesis and Microstructure Characterizations

Figures 3(a) and 3(b) show the overall view of the microstructure of the CuO grown on the top of the copper meshes. The copper oxide nanowires protruded almost vertically from the copper substrate. The direct vapor-solid (VS) mechanism had been proposed to explain the growth mechanism in which the cupric oxide was formed initially and served as the precursor for further being oxidized to CuO by maintaining enough oxide vapor pressure at a temperature above 400°C [19]. As observed in Figure 3(b), the as-prepared CuO nanowires have a length ranging from a few microns to 40 μm and a diameter of about 100 nm.

(a)

(b)

(c)

(d)

Figure 3: SEM images of ((a)-(b)) pure CuO nanowires and ((c)-(d)) CuO-In₂O₃ core-shell nanowires with different magnifications.

Figures 3(c) and 3(d) show the SEM images of the CuO-In₂O₃ composite nanowires. X-ray energy spectrum of the CuO-In₂O₃ core-shell nanowires (see Figure 4 and Table 1) confirmed the existence of indium oxide. Therefore, during the synthesis, the In(OAc)₃ which has a higher decomposition point (800°C) could be converted to the milky, amorphous indium hydroxide with lower decomposition point (600°C) according to

This amorphous indium oxide would be expected to uniformly adhere to the surface of CuO nanowire during the dip-coating and subsequently was heat-treated at 600°C to be transformed into the oxide according to the reaction:

As shown in Figures 3(c) and 3(d), after the thermal treatment, the CuO nanowire core remained leading to a successful formation of the CuO-In₂O₃ micro-p-n heterojunction.

Table 1: Summary of elemental composition of CuO-In₂O₃ analyzed in Figure 5. (C* residuals might be from the background or in the sample.)

Chemical elements
Weight percentage
Atom percentage

C*
2.85
9.33

O
18.67
45.90

Cu
64.67
40.04

In
13.81
4.73

Sum
100.00
100

Figure 4: Elemental analysis of the CuO-In₂O₃ core-shell nanowire by EDX.

3.2. Sensing Properties

For a metal oxide semiconductor-type gas sensor, the sensing mechanism is involved with the catalytical combustion of the reducing gases with the preadsorbed oxygen on the oxide surface. The form of the adsorbed oxygen on oxide is dependent upon the operating temperature. At elevated temperatures above 200°C, the preadsorbed oxygen at the surface of the oxide would extract electrons from the surface layer (known as Debye layer) usually forming O²⁻. Therefore, the reaction below could occur during the sensing process:

The released electrons would then go back to the surface conduction band of the oxide leading to the change of the resistance. This forms the basics of such type of gas sensors. For a p-type sensing oxide, the hole would be neutralized with the released electrons from the desorbed oxygen ions leading to an increase in the resistance while for an n-type oxide the resistance would decrease due to the increased electron concentrations.

Figure 5 indicates the sensitivity of CuO nanowires gas sensor to carbon monoxide within a concentration range from 60 ppm to 1100 ppm at three temperatures: 200°C, 250°C, and 300°C. The sensitivity of the sensor to CO was largest at 300°C. The sensitivity at 300°C has a relationship with the CO concentrations according to the following equation (also see inset of figure):

Figure 5: Sensitivity of pure CuO nanowires based gas sensor to carbon monoxide at different temperatures. Inset is the fitting results for the curve at 300°C.

Figure 6 shows a comparison of the response curve and sensitivity plot of the CuO nanowire based sensor to CO and propane at 300°C. The response time and recovery time of the sensor to CO are approximately 25 s and 65 s, respectively. The sensor showed a higher sensitivity relative to that to propane as shown in Figure 6(b).

(a)

(b)

Figure 6: (a) Response curve and (b) sensitivity plot of CuO nanowires based sensor to H₂, C₃H₈, and CO at 300°C.

Figures 7(a)–7(f) show the response of the CuO-In₂O₃ core-shell p-n junction nanowire based sensor to different reducing gases such as CO, hydrogen, and propane at 300°C. The response of the pure CuO based sensor was shown for the comparisons. Figures 7(a) and 7(b) show that, with the decoration of the n-type In₂O₃ nanoparticles, the resistance of the core-shell nanowire increased in presence of the reducing gases still showing a p-type conduction. This indicated that the gas sensing properties were still dominated by the CuO nanowire.

(a)

(b)

(c)

(d)

(e)

(f)

Figure 7: Comparison of response and sensitivity of CuO and CuO-In₂O₃ composite nanowire gas sensor to different gases at 300°C. ((a)-(b)) CO; ((c)-(d)) H₂; ((e)-(f)); C₃H₈.

As shown in Figures 7(a) and 7(b), the sensitivity of the CuO-In₂O₃ based sensor to CO and H₂ at 300°C decreased relative to that shown by the pure CuO based sensor. However, as shown in Figures 7(c)–7(f), the sensitivity of the CuO-In₂O₃ composite based sensor to propane was significantly enhanced. More obviously, the response time of the CuO-In₂O₃ composite nanowire gas sensor to propane is significantly shortened: only about 12 s.

The copper oxide has been reported to be doped with different metal nanomaterials (oxide) to form a donor-type or acceptor-type level to improve its gas sensing performance, increasing its sensitivity or selectivity [26–28]. p-n junction has also been adopted in literature to particularly enhance the sensitivity of the gas sensors by using the difference in the opposite response of the p and n sensing materials to reducing gases [26–28]. Therefore, the enhanced sensitivity of the CuO-In₂O₃ based sensor to propane could be attributed to p-n microheterojunction in which the oxygen adsorption was enhanced, thus enhancing reactions (5)-(6) and releasing more electrons during sensing process as suggested in the literature. However, the decrease in the sensitivity to CO and hydrogen also indicated that the catalytic role played by the In₂O₃ nanoparticles could be responsible [26–28]. The coated In₂O₃ seems to be suppressing the catalytic oxidation of CO and hydrogen with oxygen (reactions (4)-(5)) at the surface of CuO. However, the reasons are still not certain and need more investigations.

4. Conclusion

The CuO-In₂O₃ core-shell nanowire was prepared using a two-step assembly method: thermal oxidation of Cu meshes to form the CuO nanowire core followed with a dip-coating method forming the In₂O₃ nanoparticle shell on the surface of CuO. The semiconductor-type sensor using the CuO-In₂O₃ core-shell nanowires showed an enhanced response to hydrogen and propane which could be attributed to the enhanced adsorption of oxygen induced by the p-n microheterojunction while a suppressed response to CO was also observed which could be due to the fact that the catalytic properties of CuO core to CO were reduced by the decorated In₂O₃ nanoparticle shell.

Conflict of Interests

The authors declare that there is no conflict of interests regarding the publication of this paper.

Acknowledgments

The authors thank the financial support from NSF of China (Grants no. 61001054, 61131004, 61176068, 61274076, and 61306091) and the Fundamental Research Funds for the Central Universities (Grant no. DUT12LAB04).

References

O. K. Varghese, D. Gong, M. Paulose, K. G. Ong, E. C. Dickey, and C. A. Grimes, “Extreme changes in the electrical resistance of titania nanotubes with hydrogen exposure,” Advanced Materials, vol. 15, no. 7-8, pp. 624–627, 2003.

Y. Shimizu and M. Egashira, “Basic aspects and challenges of semiconductor gas sensors,” MRS Bulletin, vol. 24, no. 6, pp. 18–24, 1999.

X.-J. Huang and Y.-K. Choi, “Chemical sensors based on nanostructured materials,” Sensors and Actuators B, vol. 122, no. 2, pp. 659–671, 2007.

N. Yamazoe, “New approaches for improving semiconductor gas sensors,” Sensors and Actuators B, vol. 5, no. 1–4, pp. 7–19, 1991.

J. Rockenberger, E. C. Scher, and A. P. Alivisatos, “A new nonhydrolytic single-precursor approach to surfactant-capped nanocrystals of transition metal oxides,” Journal of the American Chemical Society, vol. 121, no. 49, pp. 11595–11596, 1999.

E. Comini, “Metal oxide nano-crystals for gas sensing,” Analytica Chimica Acta, vol. 568, no. 1-2, pp. 28–40, 2006.

S. R. Morrison, “Semiconductor gas sensors,” Sensors and Actuators, vol. 2, no. C, pp. 329–341, 1981.

G. Wang, Y. Wei, W. Zhang, X. Zhang, B. Fang, and L. Wang, “Enzyme-free amperometric sensing of glucose using Cu-CuO nanowire composites,” Microchimica Acta, vol. 168, no. 1-2, pp. 87–92, 2010.

W. Jia, M. Guo, Z. Zheng et al., “Vertically aligned CuO nanowires based electrode for amperometric detection of hydrogen peroxide,” Electroanalysis, vol. 20, no. 19, pp. 2153–2157, 2008.

I.-S. Hwang, J.-K. Choi, S.-J. Kim et al., “Enhanced H₂S sensing characteristics of SnO₂ nanowires functionalized with CuO,” Sensors and Actuators B, vol. 142, no. 1, pp. 105–110, 2009.

D. Li, J. Hu, R. Wu, and J. G. Lu, “Conductometric chemical sensor based on individual CuO nanowires,” Nanotechnology, vol. 21, no. 48, Article ID 485502, 2010.

S. B. Zhang, S.-H. Wei, and A. Zunger, “Stabilization of ternary compounds via ordered arrays of defect Pairs,” Physical Review Letters, vol. 78, no. 21, pp. 4059–4062, 1997.

Y.-S. Kim, I.-S. Hwang, S.-J. Kim, C.-Y. Lee, and J.-H. Lee, “CuO nanowire gas sensors for air quality control in automotive cabin,” Sensors and Actuators B, vol. 135, no. 1, pp. 298–303, 2008.

Y.-K. Su, C.-M. Shen, H.-T. Yang, H.-L. Li, and H.-J. Gao, “Controlled synthesis of highly ordered CuO nanowire arrays by template-based sol-gel route,” Transactions of Nonferrous Metals Society of China, vol. 17, no. 4, pp. 783–786, 2007.

L. B. Chen, N. Lu, C. M. Xu, H. C. Yu, and T. H. Wang, “Electrochemical performance of polycrystalline CuO nanowires as anode material for Li ion batteries,” Electrochimica Acta, vol. 54, no. 17, pp. 4198–4201, 2009.

B. Liu and H. C. Zeng, “Mesoscale organization of CuO nanoribbons: formation of ‘dandelions’,” Journal of the American Chemical Society, vol. 126, no. 26, pp. 8124–8125, 2004.

Y. Chang and H. C. Zeng, “Controlled synthesis and self-assembly of single-crystalline CuO nanorods and nanoribbons,” Crystal Growth and Design, vol. 4, no. 2, pp. 397–402, 2004.

H. Wu, D. Lin, and W. Pan, “Fabrication, assembly, and electrical characterization of CuO nanofibers,” Applied Physics Letters, vol. 89, no. 13, Article ID 133125, 2006.

X. Jiang, T. Herricks, and Y. Xia, “CuO nanowires can be synthesized by heating copper substrates in air,” Nano Letters, vol. 2, no. 12, 2002.

Z. Zhuang, X. Su, H. Yuan, Q. Sun, D. Xiao, and M. M. F. Choi, “An improved sensitivity non-enzymatic glucose sensor based on a CuO nanowire modified Cu electrode,” Analyst, vol. 133, no. 1, pp. 126–132, 2008.

N. Chopra, B. Hu, and B. J. Hinds, “Selective growth and kinetic study of copper oxide nanowires from patterned thin-film multilayer structures,” Journal of Materials Research, vol. 22, no. 10, pp. 2691–2699, 2007.

Y. Liu, L. Liao, J. Li, and C. Pan, “From copper nanocrystalline to CuO nanoneedle array: synthesis, growth mechanism, and properties,” Journal of Physical Chemistry C, vol. 111, no. 13, pp. 5050–5056, 2007.

J. Chen, K. Wang, L. Hartman, and W. Zhou, “H₂S detection by vertically aligned CuO nanowire array sensors,” Journal of Physical Chemistry C, vol. 112, no. 41, pp. 16017–16021, 2008.

X. Li, Y. Wang, Y. Lei, and Z. Gu, “Highly sensitive H₂S sensor based on template-synthesized CuO nanowires,” RSC Advances, vol. 2, no. 6, pp. 2302–2307, 2012.

W. Wang, Z. Liu, Y. Liu, C. Xu, C. Zheng, and G. Wang, “A simple wet-chemical synthesis and characterization of CuO nanorods,” Applied Physics A, vol. 76, no. 3, pp. 417–420, 2003.

Y. Shimizu, N. Nakashima, T. Hyodo, and M. Egashira, “NOx sensing properties of varistor-type gas sensors consisting of micro p-n junctions,” Journal of Electroceramics, vol. 6, no. 3, pp. 209–217, 2001.

C. W. Na, H.-S. Woo, I.-D. Kim, and J.-H. Lee, “Selective detection of NO₂ and C₂H₅OH using a Co₃O₄-decorated ZnO nanowire network sensor,” Chemical Communications, vol. 47, no. 18, pp. 5148–5150, 2011.

D. H. Yoon, J. H. Yu, and G. M. Choi, “CO gas sensing properties of ZnO–CuO composite,” Sensors and Actuators B, vol. 46, no. 1, pp. 15–23, 1998.